#------------------------------------------------------------------------------
#$Date: 2019-07-16 09:50:25 +0300 (Tue, 16 Jul 2019) $
#$Revision: 217055 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/31/7233138.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7233138
loop_
_publ_author_name
'Honghan Fei'
'Andrew D. LaForge'
'Tedmann M. Onyango'
'Jeremy C. Robins'
'Peter Y. Zavalij'
'Arthur P. Ramirez'
'Scott R. J. Oliver'
_publ_section_title
;
 Synthesis and magnetic properties of a 3-D nickel hydroxide capped by
 succinate
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              1099
_journal_page_last               1104
_journal_paper_doi               10.1039/C2TC00428C
_journal_volume                  1
_journal_year                    2013
_chemical_formula_sum            'C24 H24 Ni7 O31'
_chemical_formula_weight         1219.40
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.790(5)
_cell_angle_beta                 95.380(5)
_cell_angle_gamma                101.150(10)
_cell_formula_units_Z            2
_cell_length_a                   9.9900(12)
_cell_length_b                   11.2000(14)
_cell_length_c                   17.2000(16)
_cell_measurement_reflns_used    3660
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      45.2919
_cell_measurement_theta_min      2.8367
_cell_volume                     1878.8(4)
_computing_cell_refinement       'Bruker SAINT v7.34'
_computing_data_collection       'Bruker APEX-II v2.1-4'
_computing_data_reduction        'Bruker SAINT v7.34'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 83.33
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II'
_diffrn_measurement_method       ω/2θ-scans
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0600
_diffrn_reflns_av_sigmaI/netI    0.0420
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            59763
_diffrn_reflns_theta_full        30.00
_diffrn_reflns_theta_max         30.00
_diffrn_reflns_theta_min         1.19
_diffrn_standards_decay_%        .
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_number         .
_exptl_absorpt_coefficient_mu    3.544
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.7178
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.155
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1224
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.075
_refine_diff_density_max         1.096
_refine_diff_density_min         -1.143
_refine_diff_density_rms         0.131
_refine_ls_extinction_coef       0.00040(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.251
_refine_ls_hydrogen_treatment    censtr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     583
_refine_ls_number_reflns         10928
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.251
_refine_ls_R_factor_all          0.0501
_refine_ls_R_factor_gt           0.0477
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0196P)²+5.5678P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1055
_refine_ls_wR_factor_ref         0.1066
_reflns_number_gt                10605
_reflns_number_total             10928
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            J-Mat-Chem-C-2013-1-1099.cif
_cod_data_source_block           shelxl
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7233138
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 0.38240(4) 0.67199(4) 0.21499(2) 0.01206(9) Uani 1 1 d . . .
Ni2 Ni 0.11199(4) 0.50641(4) 0.17101(2) 0.00967(8) Uani 1 1 d . . .
Ni3 Ni 0.02888(4) 0.26038(4) 0.25014(2) 0.01141(9) Uani 1 1 d . . .
Ni4 Ni 0.0000 0.5000 0.0000 0.00950(11) Uani 1 2 d S . .
Ni5 Ni -0.07112(4) 0.01176(4) 0.32483(2) 0.00982(8) Uani 1 1 d . . .
Ni6 Ni -0.32804(4) -0.14417(4) 0.25387(2) 0.01322(9) Uani 1 1 d . . .
Ni7 Ni 0.0000 0.0000 0.5000 0.00956(11) Uani 1 2 d S . .
Ni8 Ni 0.02915(4) -0.23911(4) 0.25154(2) 0.01364(9) Uani 1 1 d . . .
O1 O 0.0918(2) -0.0141(2) 0.39958(12) 0.0117(4) Uani 1 1 d . . .
O2 O 0.0201(2) 0.1807(2) 0.48877(13) 0.0134(4) Uani 1 1 d . . .
O3 O 0.1737(2) 0.0220(2) 0.57684(13) 0.0121(4) Uani 1 1 d . . .
O6 O -0.4259(3) -0.1430(3) 0.00333(17) 0.0289(6) Uani 1 1 d . . .
O7 O -0.0160(2) 0.1935(2) 0.35870(12) 0.0127(4) Uani 1 1 d . . .
O8 O 0.0392(2) 0.0761(2) 0.23530(13) 0.0128(4) Uani 1 1 d . . .
O9 O -0.1312(2) -0.1642(2) 0.29247(13) 0.0130(4) Uani 1 1 d . . .
O10 O -0.2504(2) 0.0438(2) 0.26326(13) 0.0127(4) Uani 1 1 d . . .
O11 O 0.3749(2) 0.1279(2) 0.62885(13) 0.0145(4) Uani 1 1 d . . .
O12 O -0.2640(3) -0.1357(2) 0.14227(14) 0.0189(5) Uani 1 1 d . . .
O13 O -0.0037(3) 0.6156(2) 0.32557(15) 0.0206(5) Uani 1 1 d . . .
O14 O 0.0757(3) -0.0951(2) 0.17876(14) 0.0178(5) Uani 1 1 d . . .
O15 O 0.2318(3) 0.3059(2) 0.28355(14) 0.0161(5) Uani 1 1 d . . .
O16 O 0.0184(2) 0.4439(2) 0.26548(13) 0.0132(4) Uani 1 1 d . . .
O17 O 0.0629(2) 0.3213(2) 0.13900(12) 0.0126(4) Uani 1 1 d . . .
O18 O -0.1719(2) 0.2243(2) 0.21269(14) 0.0161(5) Uani 1 1 d . . .
O19 O 0.2982(2) 0.4854(2) 0.22861(13) 0.0129(4) Uani 1 1 d . . .
O20 O 0.1796(2) 0.6870(2) 0.19699(13) 0.0121(4) Uani 1 1 d . . .
O21 O 0.1869(2) 0.5312(2) 0.06497(12) 0.0115(4) Uani 1 1 d . . .
O22 O 0.0689(2) 0.4817(2) -0.10705(12) 0.0115(4) Uani 1 1 d . . .
O23 O 0.3757(3) 0.7089(2) 0.33565(14) 0.0199(5) Uani 1 1 d . . .
O24 O 0.5888(2) 0.6742(2) 0.24402(14) 0.0152(4) Uani 1 1 d . . .
O25 O -0.5301(2) -0.1462(2) 0.21074(14) 0.0160(5) Uani 1 1 d . . .
O26 O 0.3986(2) 0.6330(2) 0.09954(13) 0.0146(4) Uani 1 1 d . . .
O27 O -0.0167(2) 0.3214(2) 0.01270(13) 0.0133(4) Uani 1 1 d . . .
O28 O -0.6135(3) -0.0655(3) 0.10205(16) 0.0258(6) Uani 1 1 d . . .
O29 O 0.7042(3) 0.6199(3) 0.35049(16) 0.0246(6) Uani 1 1 d . . .
O30 O 0.3679(12) -0.1857(11) 0.6087(6) 0.033(4) Uani 0.281(12) 1 d P . .
O31 O 0.6549(5) 0.6119(4) 0.5021(2) 0.0431(14) Uani 0.848(13) 1 d P . .
O32 O 0.3742(5) 0.6350(4) 0.4932(2) 0.0402(15) Uani 0.773(12) 1 d P . .
O35 O 0.1266(3) 0.3214(2) -0.16399(14) 0.0177(5) Uani 1 1 d . . .
O37 O 0.1855(3) -0.1489(2) 0.33818(14) 0.0180(5) Uani 1 1 d . . .
C1 C 0.2948(3) 0.0804(3) 0.57094(18) 0.0133(6) Uani 1 1 d . . .
C2 C 0.3414(3) 0.0893(3) 0.48963(19) 0.0177(6) Uani 1 1 d . . .
H1 H 0.4400 0.1272 0.4935 0.021 Uiso 1 1 calc R . .
H2 H 0.2906 0.1434 0.4590 0.021 Uiso 1 1 calc R . .
C3 C 0.3199(4) -0.0346(4) 0.4454(2) 0.0203(7) Uani 1 1 d . . .
H3 H 0.3990 -0.0344 0.4147 0.024 Uiso 1 1 calc R . .
H4 H 0.3209 -0.0987 0.4844 0.024 Uiso 1 1 calc R . .
C4 C 0.1898(3) -0.0697(3) 0.39053(18) 0.0141(6) Uani 1 1 d . . .
C9 C 0.0063(3) 0.2404(3) 0.42820(17) 0.0121(5) Uani 1 1 d . . .
C10 C 0.0142(4) 0.3753(3) 0.43942(19) 0.0188(7) Uani 1 1 d . . .
H5 H 0.1082 0.4182 0.4317 0.023 Uiso 1 1 calc R . .
H6 H -0.0021 0.3924 0.4940 0.023 Uiso 1 1 calc R . .
C11 C -0.0894(4) 0.4277(3) 0.38348(18) 0.0146(6) Uani 1 1 d . . .
H7 H -0.1594 0.3598 0.3586 0.018 Uiso 1 1 calc R . .
H8 H -0.1369 0.4793 0.4141 0.018 Uiso 1 1 calc R . .
C12 C -0.0205(3) 0.5026(3) 0.32065(18) 0.0135(6) Uani 1 1 d . . .
C13 C 0.0789(3) 0.0165(3) 0.18029(18) 0.0132(6) Uani 1 1 d . . .
C14 C 0.1282(4) 0.0877(3) 0.11110(19) 0.0154(6) Uani 1 1 d . . .
H9 H 0.1690 0.0355 0.0770 0.019 Uiso 1 1 calc R . .
H10 H 0.2004 0.1586 0.1297 0.019 Uiso 1 1 calc R . .
C15 C 0.0097(4) 0.1327(3) 0.06362(19) 0.0174(6) Uani 1 1 d . . .
H11 H 0.0105 0.1111 0.0077 0.021 Uiso 1 1 calc R . .
H12 H -0.0784 0.0900 0.0807 0.021 Uiso 1 1 calc R . .
C16 C 0.0184(3) 0.2685(3) 0.07258(18) 0.0118(5) Uani 1 1 d . . .
C17 C -0.2658(3) 0.1363(3) 0.22306(18) 0.0137(6) Uani 1 1 d . . .
C18 C -0.4056(4) 0.1480(4) 0.1851(3) 0.0280(9) Uani 1 1 d . . .
H13 H -0.4076 0.1316 0.1282 0.034 Uiso 1 1 calc R . .
H14 H -0.4157 0.2335 0.1923 0.034 Uiso 1 1 calc R . .
C19 C 0.3202(3) 0.3958(3) 0.27067(18) 0.0138(6) Uani 1 1 d . . .
C20 C 0.4638(4) 0.3977(3) 0.3084(2) 0.0234(8) Uani 1 1 d . . .
H15 H 0.4749 0.3126 0.3163 0.028 Uiso 1 1 calc R . .
H16 H 0.4735 0.4383 0.3607 0.028 Uiso 1 1 calc R . .
C21 C 0.5802(4) 0.4617(3) 0.2625(2) 0.0202(7) Uani 1 1 d . . .
H17 H 0.6578 0.4184 0.2694 0.024 Uiso 1 1 calc R . .
H18 H 0.5476 0.4577 0.2062 0.024 Uiso 1 1 calc R . .
C22 C 0.6300(3) 0.5943(3) 0.2891(2) 0.0158(6) Uani 1 1 d . . .
C24 C -0.5623(3) -0.0564(3) 0.1711(2) 0.0170(6) Uani 1 1 d . . .
C25 C -0.5295(4) 0.0661(3) 0.2141(2) 0.0233(7) Uani 1 1 d . . .
H19 H -0.5110 0.0542 0.2707 0.028 Uiso 1 1 calc R . .
H20 H -0.6097 0.1061 0.2065 0.028 Uiso 1 1 calc R . .
C29 C 0.3083(3) 0.5793(3) 0.04999(18) 0.0126(6) Uani 1 1 d . . .
C30 C 0.3393(3) 0.5645(3) -0.03412(19) 0.0152(6) Uani 1 1 d . . .
H21 H 0.4395 0.5882 -0.0367 0.018 Uiso 1 1 calc R . .
H22 H 0.2948 0.6206 -0.0669 0.018 Uiso 1 1 calc R . .
C31 C 0.2899(3) 0.4338(3) -0.06794(19) 0.0149(6) Uani 1 1 d . . .
H23 H 0.3595 0.4142 -0.1008 0.018 Uiso 1 1 calc R . .
H24 H 0.2848 0.3772 -0.0241 0.018 Uiso 1 1 calc R . .
C32 C 0.1519(3) 0.4099(3) -0.11654(18) 0.0124(5) Uani 1 1 d . . .
H61 H -0.409(8) -0.079(7) -0.032(5) 0.08(2) Uiso 1 1 d . . .
H62 H -0.494(10) -0.145(9) 0.022(6) 0.11(4) Uiso 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O26 Ni1 O20 94.49(9) . .
O26 Ni1 O25 95.07(10) . 1_665
O20 Ni1 O25 98.36(9) . 1_665
O26 Ni1 O24 91.56(10) . .
O20 Ni1 O24 172.70(10) . .
O25 Ni1 O24 77.00(9) 1_665 .
O26 Ni1 O23 176.91(10) . .
O20 Ni1 O23 88.48(9) . .
O25 Ni1 O23 85.28(10) 1_665 .
O24 Ni1 O23 85.53(10) . .
O26 Ni1 O19 88.81(9) . .
O20 Ni1 O19 83.43(9) . .
O25 Ni1 O19 175.58(9) 1_665 .
O24 Ni1 O19 100.80(9) . .
O23 Ni1 O19 90.73(10) . .
O26 Ni1 Ni2 79.13(7) . .
O20 Ni1 Ni2 42.70(6) . .
O25 Ni1 Ni2 138.88(7) 1_665 .
O24 Ni1 Ni2 143.12(7) . .
O23 Ni1 Ni2 102.62(7) . .
O19 Ni1 Ni2 44.05(6) . .
O16 Ni2 O20 103.67(9) . .
O16 Ni2 O21 166.93(9) . .
O20 Ni2 O21 89.23(9) . .
O16 Ni2 O22 93.43(9) . 2_565
O20 Ni2 O22 97.97(9) . 2_565
O21 Ni2 O22 82.52(9) . 2_565
O16 Ni2 O19 89.12(9) . .
O20 Ni2 O19 85.13(9) . .
O21 Ni2 O19 94.16(9) . .
O22 Ni2 O19 175.39(9) 2_565 .
O16 Ni2 O17 81.23(9) . .
O20 Ni2 O17 173.69(9) . .
O21 Ni2 O17 86.06(9) . .
O22 Ni2 O17 85.59(9) 2_565 .
O19 Ni2 O17 91.02(9) . .
O16 Ni2 Ni1 112.13(7) . .
O20 Ni2 Ni1 43.40(6) . .
O21 Ni2 Ni1 78.69(6) . .
O22 Ni2 Ni1 136.49(6) 2_565 .
O19 Ni2 Ni1 45.16(6) . .
O17 Ni2 Ni1 131.19(7) . .
O18 Ni3 O15 176.40(9) . .
O18 Ni3 O17 86.95(9) . .
O15 Ni3 O17 90.13(9) . .
O18 Ni3 O7 89.98(9) . .
O15 Ni3 O7 92.98(9) . .
O17 Ni3 O7 176.68(9) . .
O18 Ni3 O16 89.18(10) . .
O15 Ni3 O16 88.23(10) . .
O17 Ni3 O16 79.85(9) . .
O7 Ni3 O16 101.39(9) . .
O18 Ni3 O8 90.85(10) . .
O15 Ni3 O8 91.74(10) . .
O17 Ni3 O8 100.41(9) . .
O7 Ni3 O8 78.35(9) . .
O16 Ni3 O8 179.73(9) . .
O27 Ni4 O27 180.00(12) . 2_565
O27 Ni4 O22 89.17(9) . .
O27 Ni4 O22 90.83(9) 2_565 .
O27 Ni4 O22 90.83(9) . 2_565
O27 Ni4 O22 89.17(9) 2_565 2_565
O22 Ni4 O22 180.0 . 2_565
O27 Ni4 O21 90.32(9) . .
O27 Ni4 O21 89.68(9) 2_565 .
O22 Ni4 O21 97.60(9) . .
O22 Ni4 O21 82.40(9) 2_565 .
O27 Ni4 O21 89.68(9) . 2_565
O27 Ni4 O21 90.32(9) 2_565 2_565
O22 Ni4 O21 82.40(9) . 2_565
O22 Ni4 O21 97.60(9) 2_565 2_565
O21 Ni4 O21 180.0 . 2_565
O9 Ni5 O8 101.14(9) . .
O9 Ni5 O1 94.85(9) . .
O8 Ni5 O1 96.56(9) . .
O9 Ni5 O3 89.04(9) . 2_556
O8 Ni5 O3 169.82(9) . 2_556
O1 Ni5 O3 82.43(9) . 2_556
O9 Ni5 O7 178.04(10) . .
O8 Ni5 O7 80.09(9) . .
O1 Ni5 O7 86.50(9) . .
O3 Ni5 O7 89.73(9) 2_556 .
O9 Ni5 O10 88.10(9) . .
O8 Ni5 O10 90.59(9) . .
O1 Ni5 O10 171.58(9) . .
O3 Ni5 O10 89.75(9) 2_556 .
O7 Ni5 O10 90.36(9) . .
O9 Ni5 Ni6 44.34(7) . .
O8 Ni5 Ni6 106.88(7) . .
O1 Ni5 Ni6 135.47(7) . .
O3 Ni5 Ni6 80.39(6) 2_556 .
O7 Ni5 Ni6 133.89(7) . .
O10 Ni5 Ni6 45.14(6) . .
O24 Ni6 O9 96.12(9) 1_445 .
O24 Ni6 O12 94.40(10) 1_445 .
O9 Ni6 O12 86.51(10) . .
O24 Ni6 O25 77.22(9) 1_445 .
O9 Ni6 O25 173.04(9) . .
O12 Ni6 O25 91.96(10) . .
O24 Ni6 O10 177.76(9) 1_445 .
O9 Ni6 O10 86.09(9) . .
O12 Ni6 O10 86.09(10) . .
O25 Ni6 O10 100.58(9) . .
O24 Ni6 O11 93.58(9) 1_445 2_556
O9 Ni6 O11 90.64(9) . 2_556
O12 Ni6 O11 171.76(10) . 2_556
O25 Ni6 O11 91.77(9) . 2_556
O10 Ni6 O11 86.01(9) . 2_556
O24 Ni6 Ni5 137.16(7) 1_445 .
O9 Ni6 Ni5 42.49(6) . .
O12 Ni6 Ni5 93.40(7) . .
O25 Ni6 Ni5 144.45(7) . .
O10 Ni6 Ni5 44.92(6) . .
O11 Ni6 Ni5 79.34(7) 2_556 .
O2 Ni7 O2 180.0 2_556 .
O2 Ni7 O1 89.20(9) 2_556 .
O2 Ni7 O1 90.80(9) . .
O2 Ni7 O1 90.80(9) 2_556 2_556
O2 Ni7 O1 89.20(9) . 2_556
O1 Ni7 O1 180.0 . 2_556
O2 Ni7 O3 91.76(9) 2_556 2_556
O2 Ni7 O3 88.24(9) . 2_556
O1 Ni7 O3 82.57(9) . 2_556
O1 Ni7 O3 97.43(9) 2_556 2_556
O2 Ni7 O3 88.24(9) 2_556 .
O2 Ni7 O3 91.76(9) . .
O1 Ni7 O3 97.43(9) . .
O1 Ni7 O3 82.57(9) 2_556 .
O3 Ni7 O3 180.0 2_556 .
O14 Ni8 O13 176.15(11) . 1_545
O14 Ni8 O9 90.89(9) . .
O13 Ni8 O9 92.34(10) 1_545 .
O14 Ni8 O35 88.11(10) . 2
O13 Ni8 O35 94.34(10) 1_545 2
O9 Ni8 O35 83.23(9) . 2
O14 Ni8 O20 85.22(9) . 1_545
O13 Ni8 O20 91.75(9) 1_545 1_545
O9 Ni8 O20 173.35(8) . 1_545
O35 Ni8 O20 91.23(9) 2 1_545
O14 Ni8 O37 89.81(10) . .
O13 Ni8 O37 87.79(10) 1_545 .
O9 Ni8 O37 95.73(9) . .
O35 Ni8 O37 177.66(10) 2 .
O20 Ni8 O37 89.66(9) 1_545 .
C4 O1 Ni5 131.7(2) . .
C4 O1 Ni7 126.66(19) . .
Ni5 O1 Ni7 95.91(9) . .
C9 O2 Ni7 129.4(2) . .
C1 O3 Ni7 130.7(2) . .
C1 O3 Ni5 129.2(2) . 2_556
Ni7 O3 Ni5 95.31(9) . 2_556
C9 O7 Ni5 128.1(2) . .
C9 O7 Ni3 133.3(2) . .
Ni5 O7 Ni3 97.32(9) . .
C13 O8 Ni5 129.0(2) . .
C13 O8 Ni3 132.4(2) . .
Ni5 O8 Ni3 97.46(10) . .
Ni5 O9 Ni6 93.16(9) . .
Ni5 O9 Ni8 112.40(11) . .
Ni6 O9 Ni8 138.75(12) . .
C17 O10 Ni5 127.7(2) . .
C17 O10 Ni6 136.0(2) . .
Ni5 O10 Ni6 89.94(9) . .
C1 O11 Ni6 127.4(2) . 2_556
C12 O13 Ni8 137.7(2) . 1_565
C13 O14 Ni8 137.7(2) . .
C19 O15 Ni3 132.2(2) . .
C12 O16 Ni2 129.7(2) . .
C12 O16 Ni3 132.3(2) . .
Ni2 O16 Ni3 97.63(10) . .
C16 O17 Ni3 129.2(2) . .
C16 O17 Ni2 130.20(19) . .
Ni3 O17 Ni2 95.92(9) . .
C17 O18 Ni3 131.9(2) . .
C19 O19 Ni2 126.8(2) . .
C19 O19 Ni1 139.8(2) . .
Ni2 O19 Ni1 90.78(9) . .
Ni2 O20 Ni1 93.90(9) . .
Ni2 O20 Ni8 110.66(10) . 1_565
Ni1 O20 Ni8 140.75(12) . 1_565
C29 O21 Ni2 128.5(2) . .
C29 O21 Ni4 133.3(2) . .
Ni2 O21 Ni4 96.18(9) . .
C32 O22 Ni4 119.93(19) . .
C32 O22 Ni2 129.7(2) . 2_565
Ni4 O22 Ni2 95.82(9) . 2_565
C22 O24 Ni6 123.4(2) . 1_665
C22 O24 Ni1 121.7(2) . .
Ni6 O24 Ni1 102.93(10) 1_665 .
C24 O25 Ni1 133.7(2) . 1_445
C24 O25 Ni6 120.8(2) . .
Ni1 O25 Ni6 101.99(10) 1_445 .
C29 O26 Ni1 128.3(2) . .
C16 O27 Ni4 127.3(2) . .
C32 O35 Ni8 139.3(2) . 2
C4 O37 Ni8 134.1(2) . .
O11 C1 O3 123.1(3) . .
O11 C1 C2 120.3(3) . .
O3 C1 C2 116.6(3) . .
C1 C2 C3 113.6(3) . .
C4 C3 C2 116.5(3) . .
O37 C4 O1 123.8(3) . .
O37 C4 C3 118.4(3) . .
O1 C4 C3 117.8(3) . .
O2 C9 O7 124.3(3) . .
O2 C9 C10 117.0(3) . .
O7 C9 C10 118.8(3) . .
C9 C10 C11 114.2(3) . .
C12 C11 C10 112.2(3) . .
O13 C12 O16 124.1(3) . .
O13 C12 C11 119.2(3) . .
O16 C12 C11 116.7(3) . .
O14 C13 O8 125.1(3) . .
O14 C13 C14 117.9(3) . .
O8 C13 C14 116.9(3) . .
C13 C14 C15 111.3(3) . .
C16 C15 C14 113.1(3) . .
O27 C16 O17 124.8(3) . .
O27 C16 C15 116.4(3) . .
O17 C16 C15 118.8(3) . .
O18 C17 O10 124.8(3) . .
O18 C17 C18 114.3(3) . .
O10 C17 C18 120.9(3) . .
C17 C18 C25 117.0(3) . .
O15 C19 O19 125.0(3) . .
O15 C19 C20 116.1(3) . .
O19 C19 C20 118.8(3) . .
C19 C20 C21 115.4(3) . .
C22 C21 C20 112.1(3) . .
O29 C22 O24 123.9(3) . .
O29 C22 C21 119.9(3) . .
O24 C22 C21 116.1(3) . .
O28 C24 O25 124.5(3) . .
O28 C24 C25 120.3(3) . .
O25 C24 C25 115.2(3) . .
C24 C25 C18 111.3(3) . .
O26 C29 O21 123.9(3) . .
O26 C29 C30 120.2(3) . .
O21 C29 C30 115.8(3) . .
C29 C30 C31 113.2(3) . .
C32 C31 C30 115.6(3) . .
O35 C32 O22 123.8(3) . .
O35 C32 C31 117.6(3) . .
O22 C32 C31 118.5(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ni1 O26 2.055(2) .
Ni1 O20 2.060(2) .
Ni1 O25 2.060(2) 1_665
Ni1 O24 2.071(2) .
Ni1 O23 2.120(3) .
Ni1 O19 2.122(2) .
Ni1 Ni2 2.9916(7) .
Ni2 O16 2.017(2) .
Ni2 O20 2.034(2) .
Ni2 O21 2.038(2) .
Ni2 O22 2.053(2) 2_565
Ni2 O19 2.080(2) .
Ni2 O17 2.090(2) .
Ni3 O18 2.010(2) .
Ni3 O15 2.019(2) .
Ni3 O17 2.074(2) .
Ni3 O7 2.077(2) .
Ni3 O16 2.092(2) .
Ni3 O8 2.099(2) .
Ni4 O27 1.992(2) .
Ni4 O27 1.992(2) 2_565
Ni4 O22 2.046(2) .
Ni4 O22 2.046(2) 2_565
Ni4 O21 2.050(2) .
Ni4 O21 2.050(2) 2_565
Ni5 O9 2.001(2) .
Ni5 O8 2.037(2) .
Ni5 O1 2.046(2) .
Ni5 O3 2.061(2) 2_556
Ni5 O7 2.064(2) .
Ni5 O10 2.089(2) .
Ni5 Ni6 2.9576(7) .
Ni6 O24 2.042(2) 1_445
Ni6 O9 2.070(2) .
Ni6 O12 2.077(3) .
Ni6 O25 2.080(2) .
Ni6 O10 2.096(2) .
Ni6 O11 2.126(2) 2_556
Ni7 O2 2.009(2) 2_556
Ni7 O2 2.009(2) .
Ni7 O1 2.048(2) .
Ni7 O1 2.048(2) 2_556
Ni7 O3 2.053(2) 2_556
Ni7 O3 2.053(2) .
Ni8 O14 2.064(2) .
Ni8 O13 2.075(2) 1_545
Ni8 O9 2.117(2) .
Ni8 O35 2.123(2) 2
Ni8 O20 2.133(2) 1_545
Ni8 O37 2.143(3) .
O1 C4 1.277(4) .
O2 C9 1.257(4) .
O3 C1 1.273(4) .
O3 Ni5 2.061(2) 2_556
O7 C9 1.281(4) .
O8 C13 1.286(4) .
O10 C17 1.280(4) .
O11 C1 1.259(4) .
O11 Ni6 2.126(2) 2_556
O13 C12 1.245(4) .
O13 Ni8 2.075(2) 1_565
O14 C13 1.244(4) .
O15 C19 1.241(4) .
O16 C12 1.279(4) .
O17 C16 1.279(4) .
O18 C17 1.249(4) .
O19 C19 1.286(4) .
O20 Ni8 2.133(2) 1_565
O21 C29 1.280(4) .
O22 C32 1.281(4) .
O22 Ni2 2.053(2) 2_565
O24 C22 1.294(4) .
O24 Ni6 2.042(2) 1_665
O25 C24 1.297(4) .
O25 Ni1 2.060(2) 1_445
O26 C29 1.238(4) .
O27 C16 1.251(4) .
O28 C24 1.242(4) .
O29 C22 1.229(4) .
O35 C32 1.247(4) .
O35 Ni8 2.123(2) 2
O37 C4 1.247(4) .
C1 C2 1.513(4) .
C2 C3 1.541(5) .
C3 C4 1.515(5) .
C9 C10 1.507(4) .
C10 C11 1.551(5) .
C11 C12 1.512(4) .
C13 C14 1.510(4) .
C14 C15 1.544(5) .
C15 C16 1.511(4) .
C17 C18 1.516(5) .
C18 C25 1.520(5) .
C19 C20 1.515(5) .
C20 C21 1.535(5) .
C21 C22 1.521(5) .
C24 C25 1.514(5) .
C29 C30 1.521(4) .
C30 C31 1.539(5) .
C31 C32 1.519(4) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
O26 Ni1 Ni2 O16 164.36(10) . . . .
O20 Ni1 Ni2 O16 -86.63(11) . . . .
O25 Ni1 Ni2 O16 -110.41(13) 1_665 . . .
O24 Ni1 Ni2 O16 86.47(14) . . . .
O23 Ni1 Ni2 O16 -13.04(10) . . . .
O19 Ni1 Ni2 O16 64.69(11) . . . .
O26 Ni1 Ni2 O20 -109.01(11) . . . .
O25 Ni1 Ni2 O20 -23.78(14) 1_665 . . .
O24 Ni1 Ni2 O20 173.10(15) . . . .
O23 Ni1 Ni2 O20 73.59(11) . . . .
O19 Ni1 Ni2 O20 151.32(13) . . . .
O26 Ni1 Ni2 O21 -7.97(9) . . . .
O20 Ni1 Ni2 O21 101.04(11) . . . .
O25 Ni1 Ni2 O21 77.26(13) 1_665 . . .
O24 Ni1 Ni2 O21 -85.86(13) . . . .
O23 Ni1 Ni2 O21 174.63(10) . . . .
O19 Ni1 Ni2 O21 -107.64(11) . . . .
O26 Ni1 Ni2 O22 -74.17(12) . . . 2_565
O20 Ni1 Ni2 O22 34.84(13) . . . 2_565
O25 Ni1 Ni2 O22 11.06(15) 1_665 . . 2_565
O24 Ni1 Ni2 O22 -152.06(14) . . . 2_565
O23 Ni1 Ni2 O22 108.43(12) . . . 2_565
O19 Ni1 Ni2 O22 -173.84(13) . . . 2_565
O26 Ni1 Ni2 O19 99.67(11) . . . .
O20 Ni1 Ni2 O19 -151.32(13) . . . .
O25 Ni1 Ni2 O19 -175.10(14) 1_665 . . .
O24 Ni1 Ni2 O19 21.78(15) . . . .
O23 Ni1 Ni2 O19 -77.73(12) . . . .
O26 Ni1 Ni2 O17 66.47(10) . . . .
O20 Ni1 Ni2 O17 175.48(12) . . . .
O25 Ni1 Ni2 O17 151.70(13) 1_665 . . .
O24 Ni1 Ni2 O17 -11.42(14) . . . .
O23 Ni1 Ni2 O17 -110.93(11) . . . .
O19 Ni1 Ni2 O17 -33.20(12) . . . .
O9 Ni5 Ni6 O24 19.11(14) . . . 1_445
O8 Ni5 Ni6 O24 107.88(12) . . . 1_445
O1 Ni5 Ni6 O24 -10.71(14) . . . 1_445
O3 Ni5 Ni6 O24 -79.45(12) 2_556 . . 1_445
O7 Ni5 Ni6 O24 -159.70(13) . . . 1_445
O10 Ni5 Ni6 O24 -178.79(14) . . . 1_445
O8 Ni5 Ni6 O9 88.77(12) . . . .
O1 Ni5 Ni6 O9 -29.82(13) . . . .
O3 Ni5 Ni6 O9 -98.57(11) 2_556 . . .
O7 Ni5 Ni6 O9 -178.81(13) . . . .
O10 Ni5 Ni6 O9 162.10(13) . . . .
O9 Ni5 Ni6 O12 -81.09(12) . . . .
O8 Ni5 Ni6 O12 7.68(10) . . . .
O1 Ni5 Ni6 O12 -110.91(11) . . . .
O3 Ni5 Ni6 O12 -179.65(9) 2_556 . . .
O7 Ni5 Ni6 O12 100.10(11) . . . .
O10 Ni5 Ni6 O12 81.01(11) . . . .
O9 Ni5 Ni6 O25 -179.25(15) . . . .
O8 Ni5 Ni6 O25 -90.48(14) . . . .
O1 Ni5 Ni6 O25 150.93(15) . . . .
O3 Ni5 Ni6 O25 82.18(14) 2_556 . . .
O7 Ni5 Ni6 O25 1.94(15) . . . .
O10 Ni5 Ni6 O25 -17.15(15) . . . .
O9 Ni5 Ni6 O10 -162.10(13) . . . .
O8 Ni5 Ni6 O10 -73.33(11) . . . .
O1 Ni5 Ni6 O10 168.08(13) . . . .
O3 Ni5 Ni6 O10 99.34(11) 2_556 . . .
O7 Ni5 Ni6 O10 19.09(12) . . . .
O9 Ni5 Ni6 O11 102.84(11) . . . 2_556
O8 Ni5 Ni6 O11 -168.40(9) . . . 2_556
O1 Ni5 Ni6 O11 73.01(11) . . . 2_556
O3 Ni5 Ni6 O11 4.27(9) 2_556 . . 2_556
O7 Ni5 Ni6 O11 -75.98(11) . . . 2_556
O10 Ni5 Ni6 O11 -95.07(11) . . . 2_556
O9 Ni5 O1 C4 50.7(3) . . . .
O8 Ni5 O1 C4 -51.1(3) . . . .
O3 Ni5 O1 C4 139.1(3) 2_556 . . .
O7 Ni5 O1 C4 -130.7(3) . . . .
O10 Ni5 O1 C4 161.0(5) . . . .
Ni6 Ni5 O1 C4 71.1(3) . . . .
O9 Ni5 O1 Ni7 -103.08(10) . . . .
O8 Ni5 O1 Ni7 155.09(9) . . . .
O3 Ni5 O1 Ni7 -14.70(9) 2_556 . . .
O7 Ni5 O1 Ni7 75.50(9) . . . .
O10 Ni5 O1 Ni7 7.2(7) . . . .
Ni6 Ni5 O1 Ni7 -82.66(10) . . . .
O2 Ni7 O1 C4 -49.1(3) 2_556 . . .
O2 Ni7 O1 C4 130.9(3) . . . .
O1 Ni7 O1 C4 131(100) 2_556 . . .
O3 Ni7 O1 C4 -141.0(3) 2_556 . . .
O3 Ni7 O1 C4 39.0(3) . . . .
O2 Ni7 O1 Ni5 106.63(10) 2_556 . . .
O2 Ni7 O1 Ni5 -73.37(10) . . . .
O1 Ni7 O1 Ni5 -73(100) 2_556 . . .
O3 Ni7 O1 Ni5 14.75(9) 2_556 . . .
O3 Ni7 O1 Ni5 -165.25(9) . . . .
O2 Ni7 O2 C9 -99(100) 2_556 . . .
O1 Ni7 O2 C9 38.9(3) . . . .
O1 Ni7 O2 C9 -141.1(3) 2_556 . . .
O3 Ni7 O2 C9 -43.7(3) 2_556 . . .
O3 Ni7 O2 C9 136.3(3) . . . .
O2 Ni7 O3 C1 127.1(3) 2_556 . . .
O2 Ni7 O3 C1 -52.9(3) . . . .
O1 Ni7 O3 C1 38.1(3) . . . .
O1 Ni7 O3 C1 -141.9(3) 2_556 . . .
O3 Ni7 O3 C1 -44(100) 2_556 . . .
O2 Ni7 O3 Ni5 -76.41(10) 2_556 . . 2_556
O2 Ni7 O3 Ni5 103.59(10) . . . 2_556
O1 Ni7 O3 Ni5 -165.37(9) . . . 2_556
O1 Ni7 O3 Ni5 14.63(9) 2_556 . . 2_556
O3 Ni7 O3 Ni5 113(100) 2_556 . . 2_556
O9 Ni5 O7 C9 82(3) . . . .
O8 Ni5 O7 C9 -148.7(3) . . . .
O1 Ni5 O7 C9 -51.4(3) . . . .
O3 Ni5 O7 C9 31.0(3) 2_556 . . .
O10 Ni5 O7 C9 120.7(3) . . . .
Ni6 Ni5 O7 C9 107.3(3) . . . .
O9 Ni5 O7 Ni3 -109(3) . . . .
O8 Ni5 O7 Ni3 19.89(9) . . . .
O1 Ni5 O7 Ni3 117.17(10) . . . .
O3 Ni5 O7 Ni3 -160.40(10) 2_556 . . .
O10 Ni5 O7 Ni3 -70.65(10) . . . .
Ni6 Ni5 O7 Ni3 -84.05(11) . . . .
O18 Ni3 O7 C9 -120.8(3) . . . .
O15 Ni3 O7 C9 57.1(3) . . . .
O17 Ni3 O7 C9 -143.3(15) . . . .
O16 Ni3 O7 C9 -31.7(3) . . . .
O8 Ni3 O7 C9 148.3(3) . . . .
O18 Ni3 O7 Ni5 71.49(10) . . . .
O15 Ni3 O7 Ni5 -110.55(10) . . . .
O17 Ni3 O7 Ni5 49.0(16) . . . .
O16 Ni3 O7 Ni5 160.65(9) . . . .
O8 Ni3 O7 Ni5 -19.38(9) . . . .
O9 Ni5 O8 C13 -10.4(3) . . . .
O1 Ni5 O8 C13 85.8(3) . . . .
O3 Ni5 O8 C13 169.5(4) 2_556 . . .
O7 Ni5 O8 C13 171.1(3) . . . .
O10 Ni5 O8 C13 -98.6(3) . . . .
Ni6 Ni5 O8 C13 -55.9(3) . . . .
O9 Ni5 O8 Ni3 158.77(9) . . . .
O1 Ni5 O8 Ni3 -104.95(10) . . . .
O3 Ni5 O8 Ni3 -21.3(6) 2_556 . . .
O7 Ni5 O8 Ni3 -19.67(9) . . . .
O10 Ni5 O8 Ni3 70.59(10) . . . .
Ni6 Ni5 O8 Ni3 113.36(7) . . . .
O18 Ni3 O8 C13 98.5(3) . . . .
O15 Ni3 O8 C13 -79.0(3) . . . .
O17 Ni3 O8 C13 11.4(3) . . . .
O7 Ni3 O8 C13 -171.7(3) . . . .
O16 Ni3 O8 C13 -164(71) . . . .
O18 Ni3 O8 Ni5 -70.14(10) . . . .
O15 Ni3 O8 Ni5 112.34(10) . . . .
O17 Ni3 O8 Ni5 -157.20(9) . . . .
O7 Ni3 O8 Ni5 19.66(9) . . . .
O16 Ni3 O8 Ni5 27(21) . . . .
O8 Ni5 O9 Ni6 -102.82(9) . . . .
O1 Ni5 O9 Ni6 159.51(9) . . . .
O3 Ni5 O9 Ni6 77.19(9) 2_556 . . .
O7 Ni5 O9 Ni6 26(3) . . . .
O10 Ni5 O9 Ni6 -12.59(9) . . . .
O8 Ni5 O9 Ni8 44.03(12) . . . .
O1 Ni5 O9 Ni8 -53.64(11) . . . .
O3 Ni5 O9 Ni8 -135.96(11) 2_556 . . .
O7 Ni5 O9 Ni8 173(3) . . . .
O10 Ni5 O9 Ni8 134.25(11) . . . .
Ni6 Ni5 O9 Ni8 146.85(15) . . . .
O24 Ni6 O9 Ni5 -167.06(9) 1_445 . . .
O12 Ni6 O9 Ni5 98.88(10) . . . .
O25 Ni6 O9 Ni5 176.4(7) . . . .
O10 Ni6 O9 Ni5 12.57(9) . . . .
O11 Ni6 O9 Ni5 -73.39(10) 2_556 . . .
O24 Ni6 O9 Ni8 63.01(18) 1_445 . . .
O12 Ni6 O9 Ni8 -31.05(18) . . . .
O25 Ni6 O9 Ni8 46.5(9) . . . .
O10 Ni6 O9 Ni8 -117.36(18) . . . .
O11 Ni6 O9 Ni8 156.68(17) 2_556 . . .
Ni5 Ni6 O9 Ni8 -129.9(2) . . . .
O14 Ni8 O9 Ni5 -49.30(12) . . . .
O13 Ni8 O9 Ni5 128.61(12) 1_545 . . .
O35 Ni8 O9 Ni5 -137.30(12) 2 . . .
O20 Ni8 O9 Ni5 -103.4(7) 1_545 . . .
O37 Ni8 O9 Ni5 40.60(12) . . . .
O14 Ni8 O9 Ni6 74.79(18) . . . .
O13 Ni8 O9 Ni6 -107.30(18) 1_545 . . .
O35 Ni8 O9 Ni6 -13.21(17) 2 . . .
O20 Ni8 O9 Ni6 20.7(9) 1_545 . . .
O37 Ni8 O9 Ni6 164.69(17) . . . .
O9 Ni5 O10 C17 -142.9(3) . . . .
O8 Ni5 O10 C17 -41.7(3) . . . .
O1 Ni5 O10 C17 106.4(6) . . . .
O3 Ni5 O10 C17 128.1(3) 2_556 . . .
O7 Ni5 O10 C17 38.4(3) . . . .
Ni6 Ni5 O10 C17 -155.3(3) . . . .
O9 Ni5 O10 Ni6 12.42(9) . . . .
O8 Ni5 O10 Ni6 113.54(9) . . . .
O1 Ni5 O10 Ni6 -98.3(6) . . . .
O3 Ni5 O10 Ni6 -76.64(9) 2_556 . . .
O7 Ni5 O10 Ni6 -166.36(9) . . . .
O24 Ni6 O10 C17 -50(2) 1_445 . . .
O9 Ni6 O10 C17 139.6(3) . . . .
O12 Ni6 O10 C17 52.8(3) . . . .
O25 Ni6 O10 C17 -38.5(3) . . . .
O11 Ni6 O10 C17 -129.5(3) 2_556 . . .
Ni5 Ni6 O10 C17 151.6(4) . . . .
O24 Ni6 O10 Ni5 158(2) 1_445 . . .
O9 Ni6 O10 Ni5 -12.01(9) . . . .
O12 Ni6 O10 Ni5 -98.78(10) . . . .
O25 Ni6 O10 Ni5 169.95(9) . . . .
O11 Ni6 O10 Ni5 78.90(9) 2_556 . . .
O13 Ni8 O14 C13 -110.3(14) 1_545 . . .
O9 Ni8 O14 C13 36.9(4) . . . .
O35 Ni8 O14 C13 120.1(4) 2 . . .
O20 Ni8 O14 C13 -148.5(4) 1_545 . . .
O37 Ni8 O14 C13 -58.9(4) . . . .
O18 Ni3 O15 C19 5.9(18) . . . .
O17 Ni3 O15 C19 41.7(3) . . . .
O7 Ni3 O15 C19 -139.5(3) . . . .
O16 Ni3 O15 C19 -38.1(3) . . . .
O8 Ni3 O15 C19 142.1(3) . . . .
O20 Ni2 O16 C12 15.2(3) . . . .
O21 Ni2 O16 C12 -155.3(4) . . . .
O22 Ni2 O16 C12 -83.9(3) 2_565 . . .
O19 Ni2 O16 C12 100.0(3) . . . .
O17 Ni2 O16 C12 -168.9(3) . . . .
Ni1 Ni2 O16 C12 60.1(3) . . . .
O20 Ni2 O16 Ni3 -158.41(9) . . . .
O21 Ni2 O16 Ni3 31.1(5) . . . .
O22 Ni2 O16 Ni3 102.53(10) 2_565 . . .
O19 Ni2 O16 Ni3 -73.63(10) . . . .
O17 Ni2 O16 Ni3 17.53(9) . . . .
Ni1 Ni2 O16 Ni3 -113.51(7) . . . .
O18 Ni3 O16 C12 81.8(3) . . . .
O15 Ni3 O16 C12 -100.7(3) . . . .
O17 Ni3 O16 C12 168.9(3) . . . .
O7 Ni3 O16 C12 -8.0(3) . . . .
O8 Ni3 O16 C12 -15(21) . . . .
O18 Ni3 O16 Ni2 -104.80(10) . . . .
O15 Ni3 O16 Ni2 72.70(10) . . . .
O17 Ni3 O16 Ni2 -17.75(9) . . . .
O7 Ni3 O16 Ni2 165.39(9) . . . .
O8 Ni3 O16 Ni2 158(71) . . . .
O18 Ni3 O17 C16 -50.6(3) . . . .
O15 Ni3 O17 C16 131.6(3) . . . .
O7 Ni3 O17 C16 -28.1(17) . . . .
O16 Ni3 O17 C16 -140.3(3) . . . .
O8 Ni3 O17 C16 39.8(3) . . . .
O18 Ni3 O17 Ni2 106.75(10) . . . .
O15 Ni3 O17 Ni2 -71.14(10) . . . .
O7 Ni3 O17 Ni2 129.2(15) . . . .
O16 Ni3 O17 Ni2 17.04(9) . . . .
O8 Ni3 O17 Ni2 -162.94(9) . . . .
O16 Ni2 O17 C16 139.3(3) . . . .
O20 Ni2 O17 C16 -79.4(9) . . . .
O21 Ni2 O17 C16 -37.6(3) . . . .
O22 Ni2 O17 C16 45.2(3) 2_565 . . .
O19 Ni2 O17 C16 -131.7(3) . . . .
Ni1 Ni2 O17 C16 -108.8(3) . . . .
O16 Ni2 O17 Ni3 -17.63(9) . . . .
O20 Ni2 O17 Ni3 123.7(8) . . . .
O21 Ni2 O17 Ni3 165.43(10) . . . .
O22 Ni2 O17 Ni3 -111.79(10) 2_565 . . .
O19 Ni2 O17 Ni3 71.33(10) . . . .
Ni1 Ni2 O17 Ni3 94.18(9) . . . .
O15 Ni3 O18 C17 174.2(15) . . . .
O17 Ni3 O18 C17 138.3(3) . . . .
O7 Ni3 O18 C17 -40.5(3) . . . .
O16 Ni3 O18 C17 -141.8(3) . . . .
O8 Ni3 O18 C17 37.9(3) . . . .
O16 Ni2 O19 C19 41.4(3) . . . .
O20 Ni2 O19 C19 145.2(3) . . . .
O21 Ni2 O19 C19 -125.9(3) . . . .
O22 Ni2 O19 C19 -82.3(11) 2_565 . . .
O17 Ni2 O19 C19 -39.8(3) . . . .
Ni1 Ni2 O19 C19 164.6(3) . . . .
O16 Ni2 O19 Ni1 -123.12(9) . . . .
O20 Ni2 O19 Ni1 -19.33(9) . . . .
O21 Ni2 O19 Ni1 69.54(9) . . . .
O22 Ni2 O19 Ni1 113.2(11) 2_565 . . .
O17 Ni2 O19 Ni1 155.66(9) . . . .
O26 Ni1 O19 C19 123.8(3) . . . .
O20 Ni1 O19 C19 -141.6(3) . . . .
O25 Ni1 O19 C19 -27.5(14) 1_665 . . .
O24 Ni1 O19 C19 32.4(3) . . . .
O23 Ni1 O19 C19 -53.2(3) . . . .
Ni2 Ni1 O19 C19 -160.7(4) . . . .
O26 Ni1 O19 Ni2 -75.54(9) . . . .
O20 Ni1 O19 Ni2 19.13(9) . . . .
O25 Ni1 O19 Ni2 133.3(12) 1_665 . . .
O24 Ni1 O19 Ni2 -166.89(9) . . . .
O23 Ni1 O19 Ni2 107.52(10) . . . .
O16 Ni2 O20 Ni1 107.88(9) . . . .
O21 Ni2 O20 Ni1 -74.26(9) . . . .
O22 Ni2 O20 Ni1 -156.60(8) 2_565 . . .
O19 Ni2 O20 Ni1 19.97(9) . . . .
O17 Ni2 O20 Ni1 -32.6(8) . . . .
O16 Ni2 O20 Ni8 -40.90(12) . . . 1_565
O21 Ni2 O20 Ni8 136.95(10) . . . 1_565
O22 Ni2 O20 Ni8 54.62(11) 2_565 . . 1_565
O19 Ni2 O20 Ni8 -128.81(11) . . . 1_565
O17 Ni2 O20 Ni8 179(32) . . . 1_565
Ni1 Ni2 O20 Ni8 -148.79(14) . . . 1_565
O26 Ni1 O20 Ni2 68.65(10) . . . .
O25 Ni1 O20 Ni2 164.45(9) 1_665 . . .
O24 Ni1 O20 Ni2 -145.4(7) . . . .
O23 Ni1 O20 Ni2 -110.54(10) . . . .
O19 Ni1 O20 Ni2 -19.63(9) . . . .
O26 Ni1 O20 Ni8 -161.38(17) . . . 1_565
O25 Ni1 O20 Ni8 -65.58(18) 1_665 . . 1_565
O24 Ni1 O20 Ni8 -15.5(8) . . . 1_565
O23 Ni1 O20 Ni8 19.43(18) . . . 1_565
O19 Ni1 O20 Ni8 110.34(18) . . . 1_565
Ni2 Ni1 O20 Ni8 130.0(2) . . . 1_565
O16 Ni2 O21 C29 -135.2(4) . . . .
O20 Ni2 O21 C29 54.0(3) . . . .
O22 Ni2 O21 C29 152.2(3) 2_565 . . .
O19 Ni2 O21 C29 -31.0(3) . . . .
O17 Ni2 O21 C29 -121.8(3) . . . .
Ni1 Ni2 O21 C29 11.6(2) . . . .
O16 Ni2 O21 Ni4 59.3(4) . . . .
O20 Ni2 O21 Ni4 -111.43(10) . . . .
O22 Ni2 O21 Ni4 -13.29(9) 2_565 . . .
O19 Ni2 O21 Ni4 163.50(9) . . . .
O17 Ni2 O21 Ni4 72.77(10) . . . .
Ni1 Ni2 O21 Ni4 -153.84(8) . . . .
O27 Ni4 O21 C29 118.2(3) . . . .
O27 Ni4 O21 C29 -61.8(3) 2_565 . . .
O22 Ni4 O21 C29 29.0(3) . . . .
O22 Ni4 O21 C29 -151.0(3) 2_565 . . .
O21 Ni4 O21 C29 -116(100) 2_565 . . .
O27 Ni4 O21 Ni2 -77.45(10) . . . .
O27 Ni4 O21 Ni2 102.55(10) 2_565 . . .
O22 Ni4 O21 Ni2 -166.66(9) . . . .
O22 Ni4 O21 Ni2 13.34(9) 2_565 . . .
O21 Ni4 O21 Ni2 48(100) 2_565 . . .
O27 Ni4 O22 C32 -40.1(2) . . . .
O27 Ni4 O22 C32 139.9(2) 2_565 . . .
O22 Ni4 O22 C32 -174(100) 2_565 . . .
O21 Ni4 O22 C32 50.1(2) . . . .
O21 Ni4 O22 C32 -129.9(2) 2_565 . . .
O27 Ni4 O22 Ni2 103.02(10) . . . 2_565
O27 Ni4 O22 Ni2 -76.98(10) 2_565 . . 2_565
O22 Ni4 O22 Ni2 -31(100) 2_565 . . 2_565
O21 Ni4 O22 Ni2 -166.77(9) . . . 2_565
O21 Ni4 O22 Ni2 13.23(9) 2_565 . . 2_565
O26 Ni1 O24 C22 -114.4(3) . . . .
O20 Ni1 O24 C22 99.5(7) . . . .
O25 Ni1 O24 C22 150.7(3) 1_665 . . .
O23 Ni1 O24 C22 64.6(3) . . . .
O19 Ni1 O24 C22 -25.3(3) . . . .
Ni2 Ni1 O24 C22 -40.6(3) . . . .
O26 Ni1 O24 Ni6 102.01(11) . . . 1_665
O20 Ni1 O24 Ni6 -44.0(8) . . . 1_665
O25 Ni1 O24 Ni6 7.17(10) 1_665 . . 1_665
O23 Ni1 O24 Ni6 -79.01(11) . . . 1_665
O19 Ni1 O24 Ni6 -168.90(10) . . . 1_665
Ni2 Ni1 O24 Ni6 175.87(3) . . . 1_665
O24 Ni6 O25 C24 -154.6(3) 1_445 . . .
O9 Ni6 O25 C24 -137.7(7) . . . .
O12 Ni6 O25 C24 -60.5(3) . . . .
O10 Ni6 O25 C24 25.9(3) . . . .
O11 Ni6 O25 C24 112.2(3) 2_556 . . .
Ni5 Ni6 O25 C24 38.1(3) . . . .
O24 Ni6 O25 Ni1 7.11(10) 1_445 . . 1_445
O9 Ni6 O25 Ni1 24.0(8) . . . 1_445
O12 Ni6 O25 Ni1 101.18(11) . . . 1_445
O10 Ni6 O25 Ni1 -172.44(10) . . . 1_445
O11 Ni6 O25 Ni1 -86.17(11) 2_556 . . 1_445
Ni5 Ni6 O25 Ni1 -160.20(4) . . . 1_445
O20 Ni1 O26 C29 -30.6(3) . . . .
O25 Ni1 O26 C29 -129.4(3) 1_665 . . .
O24 Ni1 O26 C29 153.5(3) . . . .
O23 Ni1 O26 C29 134.2(18) . . . .
O19 Ni1 O26 C29 52.7(3) . . . .
Ni2 Ni1 O26 C29 9.4(3) . . . .
O27 Ni4 O27 C16 -12(100) 2_565 . . .
O22 Ni4 O27 C16 136.7(3) . . . .
O22 Ni4 O27 C16 -43.3(3) 2_565 . . .
O21 Ni4 O27 C16 39.1(3) . . . .
O21 Ni4 O27 C16 -140.9(3) 2_565 . . .
O14 Ni8 O37 C4 84.2(3) . . . .
O13 Ni8 O37 C4 -98.8(3) 1_545 . . .
O9 Ni8 O37 C4 -6.7(3) . . . .
O35 Ni8 O37 C4 57(3) 2 . . .
O20 Ni8 O37 C4 169.4(3) 1_545 . . .
Ni6 O11 C1 O3 -7.9(5) 2_556 . . .
Ni6 O11 C1 C2 173.1(2) 2_556 . . .
Ni7 O3 C1 O11 150.1(2) . . . .
Ni5 O3 C1 O11 0.9(5) 2_556 . . .
Ni7 O3 C1 C2 -30.9(4) . . . .
Ni5 O3 C1 C2 179.9(2) 2_556 . . .
O11 C1 C2 C3 127.6(3) . . . .
O3 C1 C2 C3 -51.4(4) . . . .
C1 C2 C3 C4 95.8(4) . . . .
Ni8 O37 C4 O1 -6.1(5) . . . .
Ni8 O37 C4 C3 175.6(2) . . . .
Ni5 O1 C4 O37 -20.4(5) . . . .
Ni7 O1 C4 O37 126.4(3) . . . .
Ni5 O1 C4 C3 158.0(2) . . . .
Ni7 O1 C4 C3 -55.3(4) . . . .
C2 C3 C4 O37 159.9(3) . . . .
C2 C3 C4 O1 -18.5(4) . . . .
Ni7 O2 C9 O7 -4.8(5) . . . .
Ni7 O2 C9 C10 174.0(2) . . . .
Ni5 O7 C9 O2 12.4(5) . . . .
Ni3 O7 C9 O2 -152.0(2) . . . .
Ni5 O7 C9 C10 -166.4(2) . . . .
Ni3 O7 C9 C10 29.2(5) . . . .
O2 C9 C10 C11 -140.8(3) . . . .
O7 C9 C10 C11 38.0(4) . . . .
C9 C10 C11 C12 -107.0(3) . . . .
Ni8 O13 C12 O16 22.0(6) 1_565 . . .
Ni8 O13 C12 C11 -158.8(3) 1_565 . . .
Ni2 O16 C12 O13 -1.2(5) . . . .
Ni3 O16 C12 O13 170.2(2) . . . .
Ni2 O16 C12 C11 179.6(2) . . . .
Ni3 O16 C12 C11 -9.0(4) . . . .
C10 C11 C12 O13 -105.1(4) . . . .
C10 C11 C12 O16 74.2(4) . . . .
Ni8 O14 C13 O8 -5.3(6) . . . .
Ni8 O14 C13 C14 177.1(2) . . . .
Ni5 O8 C13 O14 -12.5(5) . . . .
Ni3 O8 C13 O14 -178.0(2) . . . .
Ni5 O8 C13 C14 165.2(2) . . . .
Ni3 O8 C13 C14 -0.3(4) . . . .
O14 C13 C14 C15 110.2(3) . . . .
O8 C13 C14 C15 -67.7(4) . . . .
C13 C14 C15 C16 108.3(3) . . . .
Ni4 O27 C16 O17 5.4(5) . . . .
Ni4 O27 C16 C15 -173.0(2) . . . .
Ni3 O17 C16 O27 143.1(3) . . . .
Ni2 O17 C16 O27 -6.7(5) . . . .
Ni3 O17 C16 C15 -38.5(4) . . . .
Ni2 O17 C16 C15 171.7(2) . . . .
C14 C15 C16 O27 142.4(3) . . . .
C14 C15 C16 O17 -36.2(4) . . . .
Ni3 O18 C17 O10 0.0(5) . . . .
Ni3 O18 C17 C18 178.5(3) . . . .
Ni5 O10 C17 O18 1.5(5) . . . .
Ni6 O10 C17 O18 -141.5(3) . . . .
Ni5 O10 C17 C18 -176.9(3) . . . .
Ni6 O10 C17 C18 40.1(5) . . . .
O18 C17 C18 C25 -162.3(3) . . . .
O10 C17 C18 C25 16.3(6) . . . .
Ni3 O15 C19 O19 -1.1(5) . . . .
Ni3 O15 C19 C20 178.6(2) . . . .
Ni2 O19 C19 O15 0.2(5) . . . .
Ni1 O19 C19 O15 155.8(3) . . . .
Ni2 O19 C19 C20 -179.6(2) . . . .
Ni1 O19 C19 C20 -24.0(5) . . . .
O15 C19 C20 C21 148.5(3) . . . .
O19 C19 C20 C21 -31.7(5) . . . .
C19 C20 C21 C22 94.5(4) . . . .
Ni6 O24 C22 O29 13.9(5) 1_665 . . .
Ni1 O24 C22 O29 -122.2(3) . . . .
Ni6 O24 C22 C21 -166.6(2) 1_665 . . .
Ni1 O24 C22 C21 57.3(4) . . . .
C20 C21 C22 O29 76.4(4) . . . .
C20 C21 C22 O24 -103.1(3) . . . .
Ni1 O25 C24 O28 -36.7(5) 1_445 . . .
Ni6 O25 C24 O28 118.1(3) . . . .
Ni1 O25 C24 C25 145.0(3) 1_445 . . .
Ni6 O25 C24 C25 -60.2(4) . . . .
O28 C24 C25 C18 -72.6(4) . . . .
O25 C24 C25 C18 105.8(4) . . . .
C17 C18 C25 C24 -86.8(4) . . . .
Ni1 O26 C29 O21 -4.4(5) . . . .
Ni1 O26 C29 C30 177.1(2) . . . .
Ni2 O21 C29 O26 -9.0(5) . . . .
Ni4 O21 C29 O26 150.9(2) . . . .
Ni2 O21 C29 C30 169.5(2) . . . .
Ni4 O21 C29 C30 -30.5(4) . . . .
O26 C29 C30 C31 132.4(3) . . . .
O21 C29 C30 C31 -46.2(4) . . . .
C29 C30 C31 C32 97.1(3) . . . .
Ni8 O35 C32 O22 3.4(5) 2 . . .
Ni8 O35 C32 C31 -176.0(2) 2 . . .
Ni4 O22 C32 O35 120.3(3) . . . .
Ni2 O22 C32 O35 -8.8(5) 2_565 . . .
Ni4 O22 C32 C31 -60.3(3) . . . .
Ni2 O22 C32 C31 170.6(2) 2_565 . . .
C30 C31 C32 O35 158.2(3) . . . .
C30 C31 C32 O22 -21.2(4) . . . .
